|Supported Processes||Supported Processes|
|User Processes||User Processes|
|Warning:||This page has not been released yet.|
- The tank is currently empty. Please create a help desk ticket if you need to use the gold plating station.
- Plating rate (based on 2mA/cm2 open area) 100nm/min
- Very small features and high aspect ratios may limit plating rate because of depletion of gold ions in the feature
- Aspect ratio is normally limited by photoresist
- Typical plating thickness ranges from 0.1 to 20um. If you are plating thicker than 20um please contact a tool engineer.
- BDT-510 makeup (plating solution itself)
- BDT Brightener (an additive for improving surface finish)
- Sodium Sulphate (anhydrous) CAS # 7757-82-6
- Glass tank
- Wafter holder
- Platinum Annode on teflon holder
- Hotplate with temperature probe
- Filter and filter pump
- Programmable current source (DC)
- Digital Volt Meter
- small pieces to 6" wafers
- All substrates
|Warning:||You must use the buddy system for all chemical processing. No processing if you are alone in the lab. If the yellow warning lights are on it means that there are 2 or 1 people in the lab.|
Working with chemicals can be very dangerous. Chemicals used at this bench are some of the most hazardous in the lab. To minimize the chance of accident, make sure you always:
- Wear personal protective equipment. Required PPE at this bench is an apron, face shield, and Trionic gloves.
- Know the properties and hazards of chemicals you are working with. If you don’t know, find out by reading about them or asking staff.
- Plan the details of your process. Before you start working, plan what quantities of chemicals and sample carriers you will use. Plan how you will rinse your sample and what you will do with any waste generated. Make sure you know how the controllers work.
- Do not use this bench without proper training.
- Waste from this bench goes into the LNF’s acid waste neutralization system and then to city sewers.
- No gold plating solution can be used or disposed of here.
The Gold Plating is designated as a Metals class tool. Below is a list of approved materials for the tool. Approved means the material is allowed in the tool under normal circumstances. If a material is not listed, please create a helpdesk ticket or email firstname.lastname@example.org for any material requests or questions.
The only process utilized on this tool is DC gold plating. For resists, we have found that SPR220 is not a good plating resist. 9260, KMPR, and SU8 all make very good plating molds and can be patterned in very high aspect ratios.
Standard operating procedure
Widget text will go here.
- Read through this page and the Standard Operating Procedure above.
- Create a Helpdesk Ticket requesting training.
- A tool engineer will schedule a time for initial training.
- Practice with your mentor or another authorized user until you are comfortable with tool operation.
- Schedule a checkout session with a tool engineer via the helpdesk ticket system. If this checkout is successful, the engineer will authorize you on the tool.
- The solution is changed after 50A Hrs
- Brightener is added when the surface of the plated gold becomes rough
- If you find issues with the plating, please create a help desk ticket